Embed Size (px)
ANNOTATION TO THE LESSON № 5
ELASTOMERIC IMPRESSION MATERIALS
The impression materials discussed so far are not good enough generally for taking accurate impressions of the dental patient. The alginates arc inherently weak materials and provide poor reproduction of surface detail; agar is dimensionally unstable and only suitable if laboratory facilities arc close at hand; and the rigid impression materials cannot be removed from deep undercuts. Thus, there is still a need for an impression material that is accurate, that shows a large recoverable deformation, and has adequate long-term (dimensional stability. These goals can all be met with the elastomeric impression materials.
The elastomeric impression materials arc characterised as polymers that are used at a temperature above their glass transition temperature. Such materials become more and more fluid as their temperature is raised above their glass transition temperature, Tg.
The viscosities of the polymers that are used for impression materials are governed primarily by the molecular weight of the polymer (i.e. the length of the polymer chains) and by the presence of additives, such as fillers. Thus, we have a material that is fluid at room temperature, but that can be turned into a solid by binding the long-chain molecules together. This process of binding the chains to form a three-dimensional network is known as cross-linking and forms the basis of the liquid-to-solid transition or all the elastomeric impression materials. There are essentially three main groups of elastomeric impression materials:
ü polysulphides ü polyethers ü silicones (C-type and A-type). Each group the elastomers is classified according to its viscosity. In the table
№1 4 viscosity types of the elastomeric impression materials are presented.
Types of the elastomers (ISO4823:1992) Type (ISO)
Characteristic of viscosity ( a disc diameter in mm)
0 1 2 3
(P) putty (H) high
(M) middle (L) low
≤ 30 20 - 31 31 - 36 36 min
Polysulfide rubber (mercaptan)
Polysulfide rubbers are widely used for fixed partial denture application, due to their high accuracy and relatively low cost. These materials are useful for multiple impressions when extra time is needed. The polysulfides are supplied in tubes of base paste and catalyst paste, which are mixed together. Polysulfides are available in low, medium, and high viscosities.
Composition The base paste contains the polysulfide polymer, fillers, and plasticizers. The content of the reinforcing fillers (eg, zinc oxide, titanium dioxide, zinc sulfide, and silica) varies from 12% to 50% depending on the consistency (light, regular, or heavy). The fillers and plasticizers control the stiffness of the paste. The accelerator or catalyst paste contains lead dioxide (30%), hydrated copper oxide or organic peroxide, as a catalyst; sulfur (1% to 4%) as a promoter; and dibutyl phthalate or other nonreactive oils (17%) to form a paste. The balance of the catalyst paste is inorganic fillers used to adjust the consistency and reactivity. Those materials containing an organic peroxide may have decreased dimensional stability due to evaporation of the peroxide. Note that this is a condensation polymerization with water as a by-product. Mechanical properties
For elastic recovery, the polysulfides have values of about 96%, slightly lower than those for the other rubber impression materials (eg, silicone and polyether). Values for flow range from 0.4% to 1.9%, indicating a tendency to distort upon storage. The flow tends to be highest for the light-bodied and least for the heavy bodied materials. Light-bodied polysulfides have flexibilities of about 16%; regular bodied polysulfides have values of about 14%; and heavy-bodied polysulfides have values of about 10%. This is an advantage over the stiffer addition silicones and polyethers because removal from undercut areas is
easier. Polysulfides have the highest tear strength of the rubber materials, which allows their use in deep subgingival areas where removal is difficult. Manipulation
These materials are mixed on a mixing pad with a spatula. Equal lengths of base and catalyst are extruded on a disposable mixing pad. The components are mixed thoroughly with a stiff tapered spatula. The catalyst is dark and the base is white so thorough mixing is readily observed by lack of streaks in the mix. Adequate mixing time is 45 to 60 seconds. The working time is about 5 to 7 minutes , which is adequate considering the mixing times. Both working and setting times are shortened by higher temperatures and humidity. A value of 0.45% is given for shrinkage after 24 hours. Although this is less than that of the condensation silicones, the cast or die should be poured within 1 hour of taking the impression. Since polysulfides take longer to set than silicones, they require more chair time. They stain clothing permanently. They can be electroplated; some products can be silverplated, but copperplating is not recommended.
Advantages Advantages of polysulfides include a long working time, good tear strength, good flow before setting, good reproduction of surface detail, high flexibility for easier removal around undercuts, and lower cost compared to silicones and polyethers.
Disadvantages Disadvantages of these materials include the need to use custom-made rather than stock trays due to a greater chance of distortion, a bad odor, a tendency to run down the patient's throat due to lower viscosity, and the lead dioxide materials that stain clothing. Polysulfides must be poured within 1 hour and cannot be repoured.
Troubleshooting Sometimes problems may be encountered when using polysulfide rubber impression materials: 1. Inadequate working time. This could result from excessive humidity and/or temperature. An increase in either of these variables results in decreased working and setting times. An improper base-to-catalyst ratio could also produce inadequate working time (too much catalyst will reduce working time).
2. Distortion. A number of factors cause distortion, one of which is too much load. Because recovery after deformation is dependent on the amount and duration of loading, the impression should not be placed face down on the laboratory bench.
Improper removal from the mouth could also cause distortion of the impression; removal should be rapid because permanent deformation is a function of duration of stress. If a bubble is located just below the surface adjacent to a preparation (internal porosity), the impression may distort.
3. Loss of detail. Premature removal from the mouth may be a cause of this. Removal prior to sufficient polymerization or before the material is sufficiently elastic will result in inaccurate registration of detail. This may also be the result of incomplete mixing; failure to incorporate all the catalyst into the base will result in incomplete polymerization of portions of the surface. Movement of the tray prior to the time of removal could also cause loss of detail. The impression tray should be held firmly until the elastic stage is attained.
4. Surface bubbles or voids. These could be caused by the incorporation of air into the mix. The impression material should always be mixed carefully with only the flat surface of the blade. If the material is partially polymerized prior to insertion in the mouth, voids may occur in the impression.
Disinfection Polysulfide impressions can be disinfected by immersion in sodium
hypochlorite, iodophors, complex phenolics, glutaraldehydes, or phenolic glutaraldehydes. The manufacturer's recommendations for proper disinfection should be followed.
Silicone rubber condensation type Condensation silicone rubber impression materials are used mainly for
fixed partial denture impressions. They are ideal for single-unit inlays. These materials are supplied either as two-paste or paste-liquid catalyst systems. Condensation silicones are available in low, medium, high, and very high (putty) viscosities.
Composition The base paste usually contains a moderately high-molecular-weight
poly(dimethylsiloxane) with terminal hydroxy groups (-OH), an orthoalkylsilicate for cross-linking, and inorganic filler. A paste will contain 30% to 40% filler, whereas a putty will contain as much as 75%. The catalyst paste or liquid usually contains a metal organic ester, such as tin octoate or dibutyl tin dilaurate, and an oily diluent. A thickening agent is used when making catalyst
pastes. Sometimes a catalyst will contain both the orthoalkylsilicate and the metal organic ester. A volatile alcohol is formed as a by-product.
Mechanical properties Accepted values for the mechanical properties of these materials are given
in An average value of 99% for elastic recovery is excellent. The flow of silicones is low; most values are less than 0.1%, indicating that less distortion is likely to be caused by light pressure on standing. The silicones are stiffer than polysulfides, as indicated by lower flexibility values in The shrinkage in 24 hours ranges from 0.2% to 1.0%. About half the shrinkage takes place in the first hour, and it is greater than for polysulfides or polyethers. Polymerization and evaporation of the alcohol formed in the reaction are responsible for this high shrinkage. Accuracy is greatly improved by first taking an impression with a highly filled silicone putty and, after setting, taking a second impression with a light-bodied silicone. Thus, the final total shrinkage is lower.
Manipulation The manipulation of condensation silicones is the same as for polysulfides,
except that the silicone material may be supplied as a base paste plus a liquid catalyst. When it is supplied in this form, one drop per inch of extruded base paste is usually recommended. The setting time (6 to 8 minutes) is less than that of the polysulfides, which offers some advantage in chair time savings. Electroplating is possible. Because of the high polymerization shrinkage, the cast or die must be poured as soon as possible. Higher temperatures and humidity shorten the setting time.
1 2 3
Fig. 1 Sequence of hand mixing of silicone condensation type 0 and 1 viscosity types.
1 2 3
Fig. 2 Sequence of hand mixing of silicone condensation type 2 and 3 viscosity types
Advantages Condensation silicones are clean, pleasant materials for the patient. They
are highly elastic, and the setting time can be controlled with the amount of accelerator. The use of a putty-wash system improves accuracy and eliminates the need for a custom tray.
Disadvantages These materials tend to be inaccurate due to shrinkage on standing and
should be poured within 1 hour. They are very hydrophobic, require a very dry field, and are difficult to pour in stone.
Troubleshooting 1. Inadequate working time. This could result from excessive humidity and/or temperature. Although not as critical as polysulfide rubber, the setting times of silicone impression materials are influenced by temperature and humidity. Increases in these conditions tend to shorten both working and setting times. An improper baseto-catalyst ratio could also produce inadequate working time. Insufficient catalyst will result in prolonged setting times. Failure to polymerize in the predicted time may result from deterioration during storage. 2. Distortion. This may result from incorrect separation from impressed structures. Failure to remove the impression in a rapid, jerking motion may cause the impression to become permanently deformed. An impression can also become
distorted if there is inadequate support of the impression after removal from the mouth. It may undergo permanent deformation if allowed to rest face down on the bench. Excessive delay in pouring the cast (30 minutes or more) also may result in dimensional changes. Possible shrinkage may result from continued polymerization and vaporization of volatiles in the silicone rubber. This shrinkage can be compensated for by use of the double impression technique. A preliminary impression is made with a very highviscosity material (putty), providing space for the final impression, which is made with a low-viscosity material using the preliminary impression as the tray.
3. Loss of detail. Premature removal of the impression from the mouth could cause loss of detail. Failure to allow the impression material to set adequately will result in plastic deformation. Loss of detail also can be caused by incomplete mixing. Failure to adequately incorporate all the catalyst into the base will result in incomplete polymerization. Loss of detail can also result from movement of the tray after the impression has been seated. Failure to maintain the tray in a stable position will result in a blurred impression.
Disinfection Condensation silicone impressions can be disinfected by immersion in
sodium hypochlorite, iodophors, complex phenolics, glutaraldehydes, or phenolic glutaraldehydes. The manufacturer's recommendations for proper disinfection should be followed.
Silicone rubbers addition type
Addition silicones represent an advance in accuracy over condensation silicones. This has been achieved by a change in polymerization reactions to an addition type and the elimination of an alcohol by-product that evaporates, causing shrinkage. These materials are available as two-paste systems in four viscosities light, medium, heavy, and putty and a range of colors, allowing monitoring of the degree of mixing. Due to their high accuracy, these materials are suitable for fixed and removable partial denture impressions. They are rigid after setting and expensive, and therefore are not used for routine study models. Hydrophilic materials have been introduced that reportedly contain surfactants to improve the wetting characteristics compared to unmodified silicones. Monophase materials have been formulated with sufficient shear thinning to be used as both low-viscosity and high-viscosity materials.
Composition These materials are based on silicone prepolymers with vinyl and hydrogen
side groups, which can polymerize by addition polymerization. They are therefore called vinyl or addition silicones. The setting reaction is produced by mixing one paste containing the vinyl-poly(dimethylsiloxane) prepolymer with a second paste that contains a siloxane prepolymer with hydrogen side groups. Other reactions also occur that may release hydrogen gas, which on rare occasion can produce porosity. Some manufacturers include hydrogen absorbers in their formulations to eliminate this problem. Since no volatile by-products are produced in the reaction, addition silicones have a much greater dimensional stability than condensation silicones. Some manufacturers include a retarder for extending the working and setting times.
Mechanical properties The working and setting times of addition silicones are faster than
polysulfides; a retarder is often supplied to extend the working time. Addition silicones have excellent elasticity and show very low dimensional shrinkage upon storage. Therefore, addition silicones can be safely poured up later or sent to a dental laboratory. Addition silicones do have greater rigidity, however, and therefore it is difficult to remove the impression around undercuts, as indicated by the lower flexibility value. The tear strength of addition silicones is similar to that of condensation silicones, but less than that of polysulfides.
Manipulation Addition silicones are as pleasant to handle as condensation silicones.
Because there is the possibility of hydrogen release upon setting, finely divided palladium is added to some products to absorb the hydrogen and prevent bubbles from forming on stone die surfaces. If a product does not contain a hydrogen absorber, an hour should pass before pouring dies, and the impression should stand overnight before epoxy dies are poured. Addition silicones can be electroplated with both copper and silver. Automatic mixers that provide quick, bubble-free mixes are available with several products.
Advantages Addition silicones are highly accurate and have high dimensional stability
after setting. Recovery from deformation on removal is excellent. The material stays in the tray of reclined patients, does not stain clothing, has pleasant colors and scents, may be used with stock or custom trays, and can be copper- or
silverplated. The materials may be poured 1 week after taking the impression, and multiple pours are possible.
Disadvantages The disadvantages are that the material is expensive twice the cost of
polysulfides; is more rigid than condensation silicones and difficult to remove around undercuts; has a moderate tear strength, making removal from gingival retraction areas somewhat risky; and may release hydrogen gas on setting, producing bubbles on die surfaces if an absorber is not in the product. Hydrophobic materials are difficult to electroplate and to pour in stone. Also, sulfur in latex gloves and rubber dams can inhibit polymerization.
Troubleshooting 1. Inadequate working time. This can result from excessive temperature. As the temperature increases, the working and setting times decrease. If the impression material does not set, the catalyst may have been contaminated. The platinum containing catalyst becomes inactive after contacting certain substances, such as tin or sulfur compounds. If addition silicones are combined with condensation silicones, the material will not set. Components from these two systems are not compatible and cannot be mixed together. 2. Loss of detail. This could occur if unmodified addition silicones are used. These hydrophobic materials cannot displace any moisture or hemorrhage that is not removed prior to placement of the impression material.
3. Porosity. The stone surface may appear porous if hydrogen gas is evolved. If this is the case, it is recommended that the pouring of dies be delayed for at least 1 hour.
4. Distortion. This may occur if the polysiloxane adhesive does not provide adequate retention. Mechanical retention may be required in combination with the adhesive.
Disinfection Addition silicone impressions can be disinfected by immersion in sodium hypochlorite, iodophors, complex phenolics, glutaraldehydes, or phenolic glutaraldehydes. The manufacturer's recommendations for proper disinfection should be followed.
1 2 3
Fig. 3 Silicone condensation type 0 viscosity type (1), 3 viscosity type (2), and universal catalyst (3)
Fig. 4 Silicone addition type for hand mixing (1) and automatic mixing (2)
Polyether rubber Polyether rubbers are used for accurate impressions of a few prepared teeth
without severe undercuts. Their high stiffness and short working time restricts
their use to impressions of a few teeth. Polyethers are available in low-, medium-, and high viscosity materials.
Composition Polyethers are supplied as two-paste systems. The base paste contains low-
molecular weight polyether with ethylene-imine terminal groups, along with fillers, such as colloidal silica, and plasticizers. The catalyst paste contains an aromatic sulfonic acid ester plus a thickening agent to form a paste along with fillers. When the base paste is mixed with the catalyst paste, ionic polymerization occurs by ring opening of the ethylene-imine group and chain extension. The reaction converts the paste to a rubber .
Mechanical properties Polyethers are similar to addition silicones in properties. The early
polyethers had short working and setting times and low flexibilities. Thinners were available to increase the working time and flexibility without any significant loss of other physical or mechanical properties. However, more recent formulations have a working time of 2.5 minutes and a setting time of 4.5 minutes Shrinkage values of 0.3% in 24 hours place the polyethers at the upper end of the range for accuracy, but inferior to some addition silicones. Because this rubber absorbs water and changes dimensions, storage in water is not recommended. Elastic recovery values average 98.5%, between those for polysulfides and addition silicones. The flow of polyethers is very low and contributes to accuracy. The flexibility also is low (i.e., the stiffness is high). This quality causes some problems on removal of the impression from the mouth or the die from the impression. More rubber between the tray and the impression area is recommended to relieve this problem. Polyethers have low tear strength values.
Manipulation The manipulation of polyethers is similar to that of polysulfides and
silicones. Equal lengths of base and catalyst paste are mixed vigorously and rapidly (30 to 45 seconds), because the working time is short. They are easy to mix. The impressions can be readily silverplated to produce accurate dies. Precautions should be taken to mix the material thoroughly and to avoid contact of the catalyst with the skin or mucosa because tissue reactions have been observed. A handheld gun-type mixer that provides quick, bubble-free mixes is available for one product (Permadyne Garant, ESPE). Also, an automatic mixing device (Pentamix, ESPE) has been introduced for use with a polyether packaged in polybags (Impregum Penta).
Fig. 5 Impression taken with Impregumtm Penta polyether impression material
Advantages Advantages of polyethers include pleasant handling and ease of mixing.
These materials are more accurate than polysulfide or condensation silicone impression materials. They have good surface detail reproduction and are easily poured in stone. If kept dry, they will be dimensionally stable for up to 1 week. Disadvantages
Disadvantages include high cost, short working and setting times, and high stiffness after setting, which limit their use. Their bitter taste is objectionable to some patients. Storage of polyether impressions is critical, as they will distort if stored in water or high humidity. They cannot be left in disinfectant solutions for long periods. Troubleshooting 1. Inadequate working time. This can result from excessive temperature. An increase in temperature will decrease the working and setting times. An improper base-tocatalyst ratio (too much catalyst) will decrease the working time. 2. Tearing. The rigidity of this material may result in tearing upon removal of the impression from the mouth or of the die from the impression. Tearing may occur if the rubber thickness is inadequate (at least 4 mm).
3. Distortion. The impression may distort due to moisture absorption and/or plasticizer extraction. These phenomena may result in dimensional change when impressions are stored in high-humidity environments or are exposed to water. The use of the thinner may increase the water absorption. Delay in impression placement may cause distortion. The onset of setting will result in the formation of elastic properties, which will cause deformation upon removal from the mouth.
4. Loss of detail. This can be caused by incomplete mixing. Failure to obtain a homogeneous mix will result in incomplete polymerization. If problems are encountered with multiple dies, it may be the result of gingival tearing and/or swelling. The rigidity and the relatively low tear strength of the polyethers may result in progressive deterioration at the gingival margin of the impression. The impression may absorb enough moisture from the gypsum that multiple pours could produce swelling.
Disinfection Polyether impressions can be disinfected by immersion in sodium hypochlorite. The manufacturer's recommendations for proper disinfection should be followed.